J. Electroanal. Chem., 272 (1989) 273-215 Elsevier Sequoia S.A., Lausanne - Printed
in The Netherlands
Quartz crystal microbalance analysis Part I. Evidence of anion or cation insertion into electropolymerized conducting polymers Katsuhiko Naoi, Mary M. Lien and William H. Smyrl Corrosion Research Center, Department of Chem Eng. & Mat. Sri., University of Minnesota, 221 Church St. SE, Minneapolis, MN 55455 (U.S.A.) (Received
Utilization of the quartz crystal microbalance (QCM) in conjunction with electrochemistry allows one to determine the mass of a polymer electrode and its charge utilization simultaneously and in situ under conditions where the electrode is polarized electrochemically. This combination of measurements has already been used for the following cases; (i) electrodeposition of metals [l]; (ii) dissolution of metals (Ni , Cu and Co ); (iii) redox processes for conducting polymers (polypyrrole , polyaniline ) and a redox polymer (polyvinylferrocene ). The method is also advantageous for monitoring the mass change of conducting polymers like polypyrrole and polyaniline during electropolymerization and doping/ undoping. The emphasis in this note is on monitoring polypyrrole growth on the electrode with time, and surveying ion motion into or out of the film during the subsequent reduction. Polypyrrole films were formed with two different types of anion; one is small, the other is a large polymeric anion [7,8]. In-situ monitoring of the mass change was done using QCM gravimetry for the above two cases, and the reduction processes at the two different films were observed. During the reduction process after polymer growth, the mass measurement of the polypyrrole films showed a decrease for polypyrrole films formed with ClO,-, which is consistent with anion undoping or movement out of the film. On the other hand, the mass increased upon reduction of the film formed with poly(4-styrenesulfonate) anions, indicating that cations insert into the polymer film in order to maintain charge neutrality. 0022-0728/89/$03.50
0 1989 Elsevier Sequoia
Shear mode 6 MHz AT-cut quartz crystals obtained from Inficon (East Syracuse, NY) were used for this investigation. The crystals had vacuum deposited gold electrodes on both sides. The total projected area exposed to the solution was 0.33 cm*. The crystal oscillator circuit included a power source and an oscillator (Inficon XTC). The frequency was measured with a frequency counter (HP5384A) and measurements were sent to and stored in a personal computer (HP9816). The experiments were carried out in a 4-necked glass cell. Two of the necks were used for the gas inlet and outlet, one for the reference electrode and the last one for the counter electrode (stainless steel, large surface area). The working electrode was the conducting polymer film deposited on the Au-coated quartz crystal in contact with the solution. The quartz plate was sealed to the cell with a silicone rubber sealant. The electrode potential was controlled by a potentiostat. The working electrode was grounded through the potentiostat. The reference electrodes employed in the present work were SCE (aqueous system) and Ag/AgNO, (a&o&rile system).
l. 2500 l=..
i g200 e
0 -200 0
.. . ..
. n..w ‘.
-“.7 -1.3 -0.7 n.,
. . . . . . .
50 Km I50 MO 250 MO 350 400 450 .5al Tim/s
Fig. 1. Mass change (Am), charge (Q) and current variation as a function of time or potential during polypyrrole formation and reduction of films at a scan rate of 10 mV s-‘. (A) polypyrrole prepared in 0.2 mol drne3 pyrrole+0.2 mol dm-’ TBACIO, (aq); (Et) polypyrrole prepared in 0.01 mol dm-’ pyrrole + 0.01 mol dm - 3 poly(sodium Cstyrenesulfonate) in a&on&rile.
215 RESULTS AND DISCUSSION
Figure 1 shows the mass change, charge and current variations of polypyrrole films during cyclic voltammetry. In Fig. lA, polypyrrole was grown with a relatively small-sized anion (ClO,-); the potential was scanned from 0.2 to 0.8 V and back from 0.8 to -1.5 V. At potentials between 0.3 and 0.8 V, the polymer grew at an almost constant rate. The polymer was then reduced between 0.3 and - 1.5 V, and the cathodic charge as well as mass change (decrease) were observed. As negative charge was consumed for the reduction of the film, anions were released from the film at the same time in order to maintain charge neutrality. On the contrary, Fig. 1B shows a completely opposite behavior to the former one during the reduction process between - 0.1 and - 1.3 V. During reduction, this film, which had incorporated the large poly(4-styrenesulfonate) anions, showed a mass increase instead of a decrease. This suggests that the film incorporated cations (Na+) during reduction to the neutral state. The net weight gain may also indicate some solvent incorporation (acetonitrile), but more details of the process will be discussed in subsequent reports. The results support the observations made by Shim&u et al.  and suggest that a conducting polymer film may be made either anion-inserting or cation-inserting by choice of the anion incorporated during electropolymerization. Small anions may move in or out during the oxidation and reduction cycle, but large anions do not and cations must move out or in to maintain net charge neutrality during the cycling. Also, in the case of polypyrrole films formed with medium-sized anions (e.g., tosylate, triflate, etc.), both the anions and the cations seem to move during the redox process [9,10]. ACKNOWLEDGEMENT This work was supported financially by the Defense Advanced Research Projects Agency and the Office of Naval Research (DARPA/ONR). REFERENCES 1 M.R. Deakin and 0. Melroy, J. Electroanal. Chem., 239 (1988) 321. 2 M. Benje, M. Eier, U. Pittermann and KG. We.il, Ber. Bunsenges. Phys. Chem., 90 (1986) 435. 3 C.J. Chandler, J.-B. Ju, R. Atanasoski and W.H. Smyrl, Corrosion ‘89, NACE (New Orleans), 1989, p. 37. 4 J.H. Kaufman, K.K. Kanazawa and G.B. Street, Phys. Rev. Lett., 53 (1984) 2461. 5 D. Orata and D.A. Buttry, J. Am. Chem. Sot., 109 (1987) 3574. 6 P.T. Varineau and D.A. Buttry, J. Phys. Chem., 91 (9187) 1292; M.D. Ward, ibid., 92 (1988) 2049. 7 T. Shimidzu, A. Ohtani, T. Iyoda and K. Honda, J. Chem. Sot., Chem. Commun., (1986) 1415. 8 L.F. Warren, J.A. Walker, D.P. Anderson and C.G. Rhodes, J. Electrochem. Sot., 136 (1989) 2286. 9 K. Naoi, M.M. Lien, B.B. Owens and W.H. Smyrl, Appl. Phys. Commun., in press. 10 K. Naoi, M.M. Lien and W.H. Smyrl, Proc. of ECS Hollywood Meeting (Symp. on Lithium Batteries), Oct. 1989, to be published.